Glass generally refers to hard, brittle, transparent material, such as those used for windows, many bottles, or eyewear. Examples of such solid materials include, but are not limited to, soda-lime glass, borosilicate glass, acrylic glass, sugar glass, Muscovy-glass, or aluminium oxynitride. In the technical sense, glass is an inorganic product of fusion which has been cooled through the glass transition to a rigid condition without crystallizing. Many glasses contain silica as their main component and glass former.
In the scientific sense the term glass is often extended to all amorphous solids (and melts that easily form amorphous solids), including plastics, resins, or other silica-free amorphous solids. In addition, besides traditional melting techniques, any other means of preparation are considered, such as ion implantation, and the sol-gel method. However, glass science and physics commonly includes only inorganic amorphous solids, while plastics and similar organics are covered by polymer science, biology and further scientific disciplines.
Glass plays an essential role in science and industry. The optical and physical properties of glass make it suitable for applications such as flat glass, container glass, optics and optoelectronics material, laboratory equipment, thermal insulator (glass wool), reinforcement fiber (glass-reinforced plastic, glass fiber reinforced concrete), and art.
The term glass developed in the late Roman Empire. It was in the Roman glassmaking center at Trier, Germany, that the late-Latin term glesum originated, probably from a Germanic word for a transparent, lustrous substance.
Pure silica (SiO2) has a "glass melting point"— at a viscosity of 10 Pa·s (100 P)— of over 2300 °C (4200 °F). While pure silica can be made into glass for special applications (see fused quartz), other substances are added to common glass to simplify processing. One is sodium carbonate (Na2CO3), which lowers the melting point to about 1500 °C (2700 °F) in soda-lime glass; "soda" refers to the original source of sodium carbonate in the soda ash obtained from certain plants. However, the soda makes the glass water soluble, which is usually undesirable, so lime (calcium oxide (CaO), generally obtained from limestone), some magnesium oxide (MgO) and aluminum oxide (Al2O3) are added to provide for a better chemical durability. The resulting glass contains about 70 to 74% silica by weight and is called a soda-lime glass. Soda-lime glasses account for about 90% of manufactured glass.
As well as soda and lime, most common glass has other ingredients added to change its properties. Lead glass, such as lead crystal or flint glass, is more 'brilliant' because the increased refractive index causes noticeably more "sparkles", while boron may be added to change the thermal and electrical properties, as in Pyrex. Adding barium also increases the refractive index. Thorium oxide gives glass a high refractive index and low dispersion, and was formerly used in producing high-quality lenses, but due to its radioactivity has been replaced by lanthanum oxide in modern eye glasses. Large amounts of iron are used in glass that absorbs infrared energy, such as heat absorbing filters for movie projectors, while cerium(IV) oxide can be used for glass that absorbs UV wavelengths (biologically damaging ionizing radiation).
Two other common glass ingredients are calumite (an iron industry by-product) and "cullet" (recycled glass). The recycled glass saves on raw materials and energy. However, impurities in the cullet can lead to product and equipment failure.
Finally, fining agents such as sodium sulfate, sodium chloride, or antimony oxide are added to reduce the bubble content in the glass. Glass batch calculation is the method by which the correct raw material mixture is determined to achieve the desired glass composition.
Contemporary glass production
Following the glass batch preparation and mixing, the raw materials are transported to the furnace. Soda-lime glass for mass production is melted in gas fired units. Smaller scale furnaces for specialty glasses include electric melters, pot furnaces, and day tanks.
After melting, homogenization and refining (removal of bubbles), the glass is formed. Flat glass for windows and similar applications is formed by the float glass process, developed between 1953 and 1957 by Sir Alastair Pilkington and Kenneth Bickerstaff of the UK's Pilkington Brothers, who created a continuous ribbon of glass using a molten tin bath on which the molten glass flows unhindered under the influence of gravity. The top surface of the glass is subjected to nitrogen under pressure to obtain a polished finish. Container glass for common bottles and jars is formed by blowing and pressing methods. Further glass forming techniques are summarized in the table Glass forming techniques.
Once the desired form is obtained, glass is usually annealed for the removal of stresses. Surface treatments, coatings or lamination may follow to improve the chemical durability (glass container coatings, glass container internal treatment), strength (toughened glass, bulletproof glass, windshields), or optical properties (insulated glazing, anti-reflective coating).
Glassmaking in the laboratory
New chemical glass compositions or new treatment techniques can be initially investigated in small-scale laboratory experiments. The raw materials for laboratory-scale glass melts are often different from those used in mass production because the cost factor has a low priority. In the laboratory mostly pure chemicals are used. Care must be taken that the raw materials have not reacted with moisture or other chemicals in the environment (such as alkali oxides and hydroxides, alkaline earth oxides and hydroxides, or boron oxide), or that the impurities are quantified (loss on ignition). Evaporation losses during glass melting should be considered during the selection of the raw materials, e.g., sodium selenite may be preferred over easily evaporating SeO2. Also, more readily reacting raw materials may be preferred over relatively inert ones, such as Al(OH)3 over Al2O3. Usually, the melts are carried out in platinum crucibles to reduce contamination from the crucible material. Glass homogeneity is achieved by homogenizing the raw materials mixture (glass batch), by stirring the melt, and by crushing and re-melting the first melt. The obtained glass is usually annealed to prevent breakage during processing.
In order to make glass from materials with poor glass forming tendencies, novel techniques are used to increase cooling rate, or reduce crystal nucleation triggers. Examples of these techniques include aerodynamic levitation (the melt is cooled whilst floating in a gas stream), splat quenching, (the melt is pressed between two metal anvils) and roller quenching (the melt is poured through rollers).
Besides common silica-based glasses, many other inorganic and organic materials may also form glasses, including plastics (e.g., acrylic glass), carbon, metals, carbon dioxide (see below), phosphates, borates, chalcogenides, fluorides, germanates (glasses based on GeO2), tellurites (glasses based on TeO2), antimonates (glasses based on Sb2O3), arsenates (glasses based on As2O3), titanates (glasses based on TiO2), tantalates (glasses based on Ta2O5), nitrates, carbonates and many other substances.
Some glasses that do not include silica as a major constituent may have physico-chemical properties useful for their application in fibre optics and other specialized technical applications. These include fluoride glasses (fluorozirconates, fluoroaluminates), aluminosilicates, phosphate glasses and chalcogenide glasses.
Under extremes of pressure and temperature solids may exhibit large structural and physical changes which can lead to polyamorphic phase transitions. In 2006 Italian scientists created an amorphous phase of carbon dioxide using extreme pressure. The substance was named amorphous carbonia(a-CO2) and exhibits an atomic structure resembling that of Silica.
Physics of glass
Unsolved problems in physics: What is the nature of the transition between a fluid or regular solid and a glassy phase? What are the physical mechanisms giving rise to the general properties of glasses?
The amorphous structure of glassy Silica (SiO2). No long range order is present, however there is local ordering with respect to the tetrahedral arrangement of Oxygen (O) atoms around the Silicon (Si) atoms.
The standard definition of a glass (or vitreous solid) is a solid formed by rapid melt quenching. If the cooling is sufficiently rapid (relative to the characteristic crystallization time) then crystallization is prevented and instead the disordered atomic configuration of the supercooled liquid is frozen into the solid state at the glass transition temperature Tg. Generally, the structure of a glass exists in a metastable state with respect to its crystalline form, although in certain circumstances, for example in atactic polymers, there is no crystalline analogue of the amorphous phase. As in other amorphous solids, the atomic structure of a glass lacks any long range translational periodicity. However, due to chemical bonding characteristics glasses do possess a high degree of short-range order with respect to local atomic polyhedra. It is deemed that the bonding structure of glasses, although disordered, has the same symmetry signature (Hausdorff-Besicovitch dimensionality) as for crystalline materials.
Glass is generally classed as an amorphous solid rather than a liquid. Glass displays all the mechanical properties of a solid. The notion that glass flows to an appreciable extent over extended periods of time is not supported by empirical research or theoretical analysis (see viscosity of amorphous materials). From a more commonsense point of view, glass should be considered a solid since it is rigid according to everyday experience.
Some people consider glass to be a liquid due to its lack of a first-order phase transition where certain thermodynamic variables such as volume, entropy and enthalpy are continuous through the glass transition range. However, the glass transition may be described as analogous to a second-order phase transition where the intensive thermodynamic variables such as the thermal expansivity and heat capacity are discontinuous. Despite this, the equilibrium theory of phase transformations in solids does not entirely hold for glass, and hence the glass transition cannot be classed as one of the classical equilibrium phase transformations in solids.
Although the atomic structure of glass shares characteristics of the structure in a supercooled liquid, glass tends to behave as a solid below its glass transition temperature. A supercooled liquid behaves as a liquid, but it is below the freezing point of the material, and will crystallize almost instantly if a crystal is added as a core. The change in heat capacity at a glass transition and a melting transition of comparable materials are typically of the same order of magnitude, indicating that the change in active degrees of freedom is comparable as well. Both in a glass and in a crystal it is mostly only the vibrational degrees of freedom that remain active, whereas rotational and translational motion is arrested. This helps to explain why both crystalline and non-crystalline solids exhibit rigidity on most experimental time scales.
Behavior of antique glass
The observation that old windows are often thicker at the bottom than at the top is often offered as supporting evidence for the view that glass flows over a matter of centuries. It is then assumed that the glass was once uniform, but has flowed to its new shape, which is a property of liquid. In actuality, the likely reason for this is that when panes of glass were commonly made by glassblowers, the technique used was to spin molten glass so as to create a round, mostly flat and even plate (the crown glass process, described above). This plate was then cut to fit a window. The pieces were not, however, absolutely flat; the edges of the disk became thicker as the glass spun. When actually installed in a window frame, the glass would be placed thicker side down both for the sake of stability and to prevent water accumulating in the lead cames at the bottom of the window. Occasionally such glass has been found thinner side down or thicker on either side of the window's edge, as would be caused by carelessness at the time of installation.
Mass production of glass window panes in the early twentieth century caused a similar effect. In glass factories, molten glass was poured onto a large cooling table and allowed to spread. The resulting glass is thicker at the location of the pour, located at the center of the large sheet. These sheets were cut into smaller window panes with nonuniform thickness. Modern glass intended for windows is produced as float glass and is very uniform in thickness.
Several other points exemplify the misconception of the "cathedral glass" theory:
* Writing in the American Journal of Physics, physicist Edgar D. Zanotto states "...the predicted relaxation time for GeO2 at room temperature is 1032 years. Hence, the relaxation period (characteristic flow time) of cathedral glasses would be even longer." (1032 years is much longer than the estimated age of the Universe.)
Some glasses have a glass transition temperature close to or below room temperature. The behavior of a material that has a glass transition close to room temperature depends upon the timescale during which the material is manipulated. If the material is hit it may break like a solid glass, but if the material is left on a table for a week it may flow like a liquid. This simply means that for the fast timescale its transition temperature is above room temperature, but for the slow one it is below. The shift in temperature with timescale is not very large however, as indicated by the transition of polypropylene glycol of -72 °C and -71 °C over different timescales. To observe window glass flowing as liquid at room temperature we would have to wait a much longer time than any human can exist. Therefore it is safe to consider a glass a solid far enough below its transition temperature: Cathedral glass does not flow because its glass transition temperature is many hundreds of degrees above room temperature. Close to this temperature there are interesting time-dependent properties. One of these is known as aging. Many polymers that we use in daily life such as polystyrene and polypropylene are in a glassy state but they are not too far below their glass transition temperature as opposed to rubber which is used above its glass transition temperature. Their mechanical properties may well change over time and this is serious concern when applying these materials in construction. In general for polymers there is a relation between the glass transition temperature and the speed of the deformation.
The following table lists some physical properties of common glasses. Unless otherwise stated, the technical glass compositions and many experimentally determined properties are taken from one large study. Unless stated otherwise, the properties of fused silica (quartz glass) and germania glass are derived from the SciGlass glass database by forming the arithmetic mean of all the experimental values from different authors (in general more than 10 independent sources for quartz glass and Tg of germanium oxide glass).
Many glasses have a chemical composition which includes what are referred to as absorption centers. This may cause them to be selective in their absorption of visible lightwaves (or white light frequencies). They absorb certain portions of the visible spectrum, while reflecting others. The frequencies of the spectrum which are not absorbed are either reflected back or transmitted for our physical observation. This is what gives rise to color.
Thus, color in glass may be obtained by addition of electrically charged ions (or color centers) that are homogeneously distributed, and by precipitation of finely dispersed particles (such as in photochromic glasses). Ordinary soda-lime glass appears colorless to the naked eye when it is thin, although iron(II) oxide (FeO) impurities of up to 0.1 wt% produce a green tint which can be viewed in thick pieces or with the aid of scientific instruments. Further FeO and Cr2O3 additions may be used for the production of green bottles. Sulfur, together with carbon and iron salts, is used to form iron polysulfides and produce amber glass ranging from yellowish to almost black. Manganese dioxide can be added in small amounts to remove the green tint given by iron(II) oxide.
Optically transparent materials focus on the response of a material to incoming light waves of a range of wavelengths. Frequency selective optical filters can be utilized to alter or enhance the brightness and contrast of a digital image. Guided light wave transmission via frequency selective waveguides involves the emerging field of fiber optics and the ability of certain glassy compositions as a transmission medium for a range of frequencies simultaneously (multimode optical fiber) with little or no interference between competing wavelengths or frequencies. This resonant mode of energy and data transmission via electromagnetic (light) wave propagation, though low powered, is relatively lossless.
An optical fiber is a cylindrical dielectric waveguide that transmits light along its axis by the process of total internal reflection. The fiber consists of a core surrounded by a cladding layer. To confine the optical signal in the core, the refractive index of the core must be greater than that of the cladding. The index of refraction is a way of measuring the speed of light in a material. (Note: The index of refraction is the ratio of the speed of light in a vacuum to the speed of light in a given medium. (The index of refraction of a vacuum is therefore equal to 1, by definition). The larger the index of refraction, the more slowly light travels in that medium. Typical values for core and cladding of an optical fiber are 1.48 and 1.46, respectively.
When light traveling in a dense medium hits a boundary at a steep angle, the light will be completely reflected. This effect is used in optical fibers to confine light in the core. Light travels along the fiber bouncing back and forth off of the boundary. Because the light must strike the boundary with an angle greater than the critical angle, only light that enters the fiber within a certain range of angles will be propagated. This range of angles is called the acceptance cone of the fiber. The size of this acceptance cone is a function of the refractive index difference between the fiber's core and cladding.
Optical waveguides are used as components in integrated optical circuits (e.g. light-emitting diodes, LEDs) or as the transmission medium in local and long haul optical communication systems. Also of value to the emerging materials scientist is the sensitivity of materials to thermal radiation in the infrared (IR) portion of the EM spectrum. This infrared homing (or "heat-seeking") capability is responsible for such diverse optical phenomena as "night vision" and IR luminescence.
Naturally occurring glass, especially obsidian, has been used by many Stone Age societies across the globe for the production of sharp cutting tools and, due to its limited source areas, was extensively traded. But in general, archaeological evidence suggests that the first true glass was made in coastal north Syria, Mesopotamia or Old Kingdom Egypt. Due to Egypt's favorable environment for preservation, the majority of well-studied early glass is found in Egypt, although some of this is likely to have been imported. The earliest known glass objects, of the mid third millennium BC, were beads, perhaps initially created as accidental by-products of metal-working slags or during the production of faience, a pre-glass vitreous material made by a process similar to glazing.
During the Late Bronze Age in Egypt and Western Asia there was an explosion in glass-making technology. Archaeological finds from this period include colored glass ingots, vessels (often colored and shaped in imitation of highly prized wares of semi-precious stones) and the ubiquitous beads. The alkali of Syrian and Egyptian glass was soda ash, sodium carbonate, which can be extracted from the ashes of many plants, notably halophile seashore plants: (see saltwort). The earliest vessels were 'core-wound', produced by winding a ductile rope of glass round a shaped core of sand and clay over a metal rod, then fusing it with repeated reheatings. Threads of thin glass of different colors made with admixtures of oxides were subsequently wound around these to create patterns, which could be drawn into festoons by using metal raking tools. The vessel would then be rolled flat ('marvered') on a slab in order to press the decorative threads into its body. Handles and feet were applied separately. The rod was subsequently allowed to cool as the glass slowly annealed and was eventually removed from the center of the vessel, after which the core material was scraped out. Glass shapes for inlays were also often created in moulds. Much early glass production, however, relied on grinding techniques borrowed from stone working. This meant that the glass was ground and carved in a cold state.
By the 15th century BC extensive glass production was occurring in Western Asia and Egypt. It is thought the techniques and recipes required for the initial fusing of glass from raw materials was a closely guarded technological secret reserved for the large palace industries of powerful states. Glass workers in other areas therefore relied on imports of pre-formed glass, often in the form of cast ingots such as those found on the Ulu Burun shipwreck off the coast of Turkey.
Glass remained a luxury material, and the disasters that overtook Late Bronze Age civilisations seem to have brought glass-making to a halt. It picked up again in its former sites, in Syria and Cyprus, in the ninth century BC, when the techniques for making colorless glass were discovered. The first glassmaking "manual" dates back to ca. 650 BC. Instructions on how to make glass are contained in cuneiform tablets discovered in the library of the Assyrian king Ashurbanipal. In Egypt glass-making did not revive until it was reintroduced in Ptolemaic Alexandria. Core-formed vessels and beads were still widely produced, but other techniques came to the fore with experimentation and technological advancements. During the Hellenistic period many new techniques of glass production were introduced and glass began to be used to make larger pieces, notably table wares. Techniques developed during this period include 'slumping' viscous (but not fully molten) glass over a mould in order to form a dish and 'millefiori' (meaning 'thousand flowers') technique, where canes of multi-colored glass were sliced and the slices arranged together and fused in a mould to create a mosaic-like effect. It was also during this period that colorless or decolored glass began to be prized and methods for achieving this effect were investigated more fully.
According to Pliny the Elder, Phoenician traders were the first to stumble upon glass manufacturing techniques at the site of the Belus River. Georgius Agricola, in De re metallica, reported a traditional serendipitous "discovery" tale of familiar type:
"The tradition is that a merchant ship laden with nitrum being moored at this place, the merchants were preparing their meal on the beach, and not having stones to prop up their pots, they used lumps of nitrum from the ship, which fused and mixed with the sands of the shore, and there flowed streams of a new translucent liquid, and thus was the origin of glass."
This account is more a reflection of Roman experience of glass production, however, as white silica sand from this area was used in the production of Roman glass due to its low impurity levels.
During the first century BC glass blowing was discovered on the Syro-Palestinian coast, revolutionising the industry and laying the way for the explosion of glass production that occurred throughout the Roman world. It was the Romans who began to use glass for architectural purposes, with the discovery of clear glass (through the introduction of manganese oxide), in Alexandria ca. AD 100. Cast glass windows, albeit with poor optical qualities, thus began to appear in the most important buildings in Rome and the most luxurious villas of Herculaneum and Pompeii. Over the next 1,000 years glass making and working continued and spread through southern Europe and beyond.
Indigenous development of glass technology in South Asia may have begun in 1730 BCE. Evidence of this culture includes a red-brown glass bead along with a hoard of beads dating to that period, making it the earliest attested glass from the Indus Valley locations. Glass discovered from later sites dating from 600–300 BCE displays common color.
Chalcolithic evidence of glass has been found in Hastinapur, India. Some of the texts which mention glass in India are the Shatapatha Brahmana and Vinaya Pitaka. However, the first unmistakable evidence in large quantities, dating from the 3rd century BCE, has been uncovered from the archaeological site in Taxila, Pakistan.
By the first century C.E., glass was being used for ornaments and casing in South Asia. Contact with the Greco-Roman world added newer techniques, and Indians artisans mastered several techniques of glass molding, decorating and coloring by the succeeding centuries. The Satavahana period of India also produced short cylinders of composite glass, including those displaying a lemon yellow matrix covered with green glass.
A full discussion of Roman glass making and working can be found on the Roman glass page.
Evidence for glass making, working and use in the 5th to 8th centuries in England is discussed in the Anglo-Saxon glass page.
The Arab poet al-Buhturi (820–897) described the clarity of such glass, "Its color hides the glass as if it is standing in it without a container."
Stained glass was also first produced by Muslim architects in Southwest Asia using colored glass rather than stone. In the 8th century, the Arab chemist Jabir ibn Hayyan (Geber) scientifically described 46 original recipes for producing colored glass in Kitab al-Durra al-Maknuna (The Book of the Hidden Pearl), in addition to 12 recipes inserted by al-Marrakishi in a later edition of the book.
The parabolic mirror was first described by Ibn Sahl in his On the Burning Instruments in the 10th century, and later described again in Ibn al-Haytham's On Burning Mirrors and Book of Optics (1021). By the 11th century, clear glass mirrors were being produced in Islamic Spain. The first glass factories were also built by Muslim craftsmen in the Islamic world. The first glass factories in Christian Europe were later built in the 11th century by Muslim Egyptian craftsmen in Corinth, Greece.
Glass objects from the 7th and 8th centuries have been found on the island of Torcello near Venice. These form an important link between Roman times and the later importance of that city in the production of the material. Around 1000 AD, an important technical breakthrough was made in Northern Europe when soda glass, produced from white pebbles and burnt vegetation was replaced by glass made from a much more readily available material: potash obtained from wood ashes. From this point on, northern glass differed significantly from that made in the Mediterranean area, where soda remained in common use.
Until the 12th century, stained glass – glass to which metallic or other impurities had been added for coloring – was not widely used.
The 11th century saw the emergence in Germany of new ways of making sheet glass by blowing spheres. The spheres were swung out to form cylinders and then cut while still hot, after which the sheets were flattened. This technique was perfected in 13th century Venice.
The Crown glass process was used up to the mid-19th century. In this process, the glassblower would spin approximately 9 pounds (4 kg) of molten glass at the end of a rod until it flattened into a disk approximately 5 feet (1.5 m) in diameter. The disk would then be cut into panes.
Late medieval Northern Europe
Glass making in late medieval Northern Europe is discussed in the article on Forest glass.
The center for glassmaking from the 14th century was the island of Murano, which developed many new techniques and became the center of a lucrative export trade in dinnerware, mirrors, and other luxury items. What made Venetian Murano glass significantly different was that the local quartz pebbles were almost pure silica, and were ground into a fine clear sand that was combined with soda ash obtained from the Levant, for which the Venetians held the sole monopoly. The clearest and finest glass is tinted in two ways: firstly, a small or large amount of a natural coloring agent is ground and melted with the glass. Many of these coloring agents still exist today; for a list of coloring agents, see below. Black glass was called obsidianus after obsidian stone. A second method is apparently to produce a black glass which, when held to the light, will show the true color that this glass will give to another glass when used as a dye.
The Venetian ability to produce this superior form of glass resulted in a trade advantage over other glass producing lands. Murano’s reputation as a center for glassmaking was born when the Venetian Republic, fearing fire might burn down the city’s mostly wood buildings, ordered glassmakers to move their foundries to Murano in 1291. Murano's glassmakers were soon the island’s most prominent citizens. Glassmakers were not allowed to leave the Republic. Many took a risk and set up glass furnaces in surrounding cities and as far afield as England and the Netherlands.
Beginning in the 20th century, glass started to become highly collectible as art. Works of art in glass can be seen in a variety of museums, including the Chrysler Museum, the Museum of Glass in Tacoma, the Metropolitan Museum of Art, the Toledo Museum of Art, and Corning Museum of Glass, in Corning, NY, which houses the world's largest collection of glass art and history, with more than 45,000 objects in its collection.
Several of the most common techniques for producing glass art include: blowing, kiln-casting, fusing, slumping, pate-de-verre, flame-working, hot-sculpting and cold-working. Cold work includes traditional stained glass work as well as other methods of shaping glass at room temperature. Glass can also be cut with a diamond saw, or copper wheels embedded with abrasives, and polished to give gleaming facets; the technique used in creating Waterford crystal. Art is sometimes etched into glass via the use of acid, caustic, or abrasive substances. Traditionally this was done after the glass was blown or cast. In the 1920s a new mould-etch process was invented, in which art was etched directly into the mould, so that each cast piece emerged from the mould with the image already on the surface of the glass. This reduced manufacturing costs and, combined with a wider use of colored glass, led to cheap glassware in the 1930s, which later became known as Depression glass. As the types of acids used in this process are extremely hazardous, abrasive methods have gained popularity.
Objects made out of glass include not only traditional objects such as vessels (bowls, vases, bottles, and other containers), paperweights, marbles, beads, but an endless range of sculpture and installation art as well. Colored glass is often used, though sometimes the glass is painted, innumerable examples exist of the use of stained glass.
The Harvard Museum of Natural History has a collection of extremely detailed models of flowers made of painted glass. These were lampworked by Leopold Blaschka and his son Rudolph, who never revealed the method he used to make them. The Blaschka Glass Flowers are still an inspiration to glassblowers today.
Editor for Asisbiz: Matthew Laird Acred
Please help us to improve these articles with any additional information or photo's, if you should encounter any broken links or display errors :-(